# Modeling of Phase Transformation in Induction Hardening .Modeling of Phase Transformation in...

date post

28-Aug-2018Category

## Documents

view

218download

1

Embed Size (px)

### Transcript of Modeling of Phase Transformation in Induction Hardening .Modeling of Phase Transformation in...

64 The Open Materials Science Journal, 2010, 4, 64-73

1874-088X/10 2010 Bentham Open

Open Access

Modeling of Phase Transformation in Induction Hardening

K. Palaniradja*, N. Alagumurthi and V. Soundararajan

Department of Mechanical Engineering, Pondicherry Engineering College, Pondicherry 605 014, India

Abstract: Mechanical properties of machined components are controlled by inducing phase transformations in the outer layer

of the materials. Induction hardening is one such manufacturing process where the surface hardness is enhanced while the

core is retained with the original structure and characteristics. In this study, a mathematical model had been developed to

predict the hardness and the volume fraction of martensite present in the hardened surface. Experiments applying induction

hardening were conducted on the following specimen materials AISI 1040, AISI 4140, AISI 4340, AISI 1055, AISI 6150 and

AISI 9255. The microstructures obtained from the experiment showed a moderate phase transformation of austenite to

martensite. The hardness and the volume fraction of martensite estimated from the experiments were found to match the

results of mathematical modeling as well as the theoretical model using regression analysis.

Keywords: Modeling, phase transformation, induction hardening, volume fraction, validation

1. INTRODUCTION

Induction hardening is an important manufacturing process to control the mechanical properties of metal parts where surface hardness is enhanced while the core retains the original structure and toughness characteristics [1]. This is possible by inducing suitable phase transformation in the outer layer of the material. Two types of modification occur when phase transformation takes place while quenching. The first type called metallurgical interaction is kinetic modifi-cation which sometimes leads to a different morphology in the phase produced. The second type (commonly called transformation plasticity) is a mechanical modification related to the progress of transformation, and takes place when plastic deformation occurs under [2] stresses lower than the yield stress of the material (Denis, S., et al., 1985).

The importance of thorough knowledge of the transformation characteristics of steel in the solution of heat treatment and steel selection problems and in the explanation of stress related phenomena has long been realized. It is obvious that for the quick decisions, which are the order of the day, metallurgists and materials engineers cannot undertake expensive and time-consuming metallographic experiments to determine volume fraction of martensite and maximum hardness value obtainable, considering heating and cooling curves relevant to their actual technology and the work material. Instead, they must turn to the literature, but unfortunately the data found, i.e. the chemical composition, grain size, heating and cooling curves indicated on the existing diagrams, differ from those required [3,4]. It is felt that the most direct assistance to the materials engineers employed in heat treatment industry is to provide them with solution in the form of mathematical models to predict the hardness and volume fraction of martensite at any point in the Induction hardened zone of a given steel

*Address correspondence to this author at the Department of Mechanical

Engineering, Pondicherry Engineering College, Pondicherry-605014, India;

Tel: 91 413 2655281-287, Ext. 252,259; Fax: 91 413 2655101; E-mail:

palaniradja72@rediffmail.com

component with any composition within the allowed range for the induction hardening steel type. Hence, in this paper a mathematical modeling has been developed to predict the volume fraction of martensite and hardness for the materials considered in the current research [5].

2. MODELING OF INDUCTION HARDENING

Modeling of induction hardening is a complex issue which involves numerically solving the Maxwells equations for electromagnetic field around workpiece, coupled with heat transfer principles for modeling the product thermal process (Nemkov, V.S., and Goldstein, R., 1999). The system is inevitably highly nonlinear because of temperature dependent material properties of workpiece. In the past, more attention of numerical simulation was paid to modeling only certain aspects of the induction hardening problem; little effort has been paid to model the integrated process from heating to final hardening. Numerical simulation of the magnetic field was ever conducted. They provided valuable analysis for the magnetic vector potential which was a very important parameter for eddy current and Joule heat determination. Simulation of induction heating has been carried out and provided models for solving coupled electromagnetic/thermal analysis. Recently, quenching and phase transformation process has been simulated. And the Koistinen-Marburger law and Avrami equation was applied for determination of volume fraction of micro-constituents formed in the quench cooling process. However, few studies have been found to predict the hardness distribution using numerical simulation.

Jiankun Yuan et al., (2003) [6] developed an integrated FEA based modeling system with the capabilities to simulate the electromagnetic field induced heating process, austenite state holding processes, and severe quenching processes. This modeling system helps in determining volume fraction of micro constituent such as martensite formed in the quench cooling process, and final hardness distribution pattern in work piece. However, there is a restriction in using this model because this model involves analysis of interaction of

Modeling of Phase Transformation in Induction Hardening The Open Materials Science Journal, 2010, Volume 4 65

continuous cooling curve with Temperature Time Transformation diagram. It must be remembered that cooling curves are difficult to obtain in Induction hardening applications. This is because the exact conditions are difficult to duplicate in the laboratory (Scott Mackenzie., 2002).

This paper deals with the model, which may be considered as an extension of Yuan model, developed to predict the volume fraction of martensite theoretically. A Regression model has also been developed to estimate the Hardness in HRA for steel materials, AISI 1040, AISI 4140, AISI 4340, AISI 1055, AISI 6150 and AISI 9255. These models overcome the drawbacks in the modeling system explained above. Experimental validation of the developed model has also been presented here.

3. MATHEMATICAL MODEL TO PREDICT THE HARDNESS

In order to develop the mathematical model to predict the hardness and volume fraction of martensite for Induction hardening of steel materials (G1 Material and G2 Material), Induction hardening experiments have been conducted.

Table 1 shows the details about the operating conditions and the materials.

Table 2 shows the experimental results in the 33 Design

Matrix for the G1 and G2 Induction hardening rack materials respectively.

Regression analysis has been carried out using MATLAB and the Regression equations (Equation to predict the hardness of the materials) have been found and the same are given below:

3.1. Model Regression Analysis

AISI 1040

Coeff =

1.0000 5.5000 1.3400 15.0000 80

1.0000 5.5000 1.3400 17.5000 78

1.0000 5.5000 1.3400 20.0000 79

1.0000 5.5000 1.7200 15.0000 80

1.0000 5.5000 1.7200 17.5000 78

1.0000 5.5000 1.7200 20.0000 82

1.0000 5.5000 2.1400 15.0000 83

1.0000 5.5000 2.1400 17.5000 74

1.0000 5.5000 2.1400 20.0000 81

1.0000 7.0500 1.3400 15.0000 74

1.0000 7.0500 1.3400 17.5000 78

1.0000 7.0500 1.3400 20.0000 77

1.0000 7.0500 1.7200 15.0000 78

1.0000 7.0500 1.7200 17.5000 74

1.0000 7.0500 1.7200 20.0000 76

1.0000 7.0500 2.1400 15.0000 78

1.0000 7.0500 2.1400 17.5000 74

1.0000 7.0500 2.1400 20.0000 78

1.0000 8.5000 1.3400 15.0000 69

1.0000 8.5000 1.3400 17.5000 65

Table 1. Experimental Conditions and Work Materials

Levels Actual Code S. No. Variables Unit Notation

Low Medium High Low Medium High

1 Power potential kW/inch2 P 5.5 7.05 8.5 L1 L2 L3

2 Scan speed m/min S 1.34 1.72 2.14 L1 L2 L3

3 Quench flow rate Litres/min Q 15 17.5 20 L1 L2 L3

Design of Experiment: Factorial Design of Experiment with 3 3 Design matrix.

Regression analysis.

Material: Group 1 (Carbon content ranging from 0.35 -0.45%, Maximum HRC possible 60).

Group 2 (Carbon content ranging from 0.45 0.6%, Maximum HRC possible 65).

Material Steel Designation Chemical Composition in Percentage

AISI 1040 C-0.35%, Si-0.10%, Mn-0.60% S&P each 0.06%

AISI 4140 C-0.35%, Si-0.10%, Mn-0.50%, Cr-0.90, Mo-0.20% S&P each 0.05%

Group 1

AISI 4340 C-0.35%, Si-0.10%, Mn-0.45%, Cr-0.90%, Mo-0.20%, Ni-1.30% S&P each 0.05%

AISI 1055 C-0.45%, Si-0.10%, Mn-0.50%, S&P each 0.06% (max)

AISI 6150 C-0.50%, Si0.50%, Mn-0.50%, Cr-0.80%, V-0.15% S&P each -0.05 (each)

Group 2

AISI 9255 C-0.55%, Si1.50%, Mn-0.70%, S&P each -0.05 (max)

66 The Open Materials Science Journal, 2010, Volume 4 Palaniradja et al.

1.0000 8.5000 1.3400 20.0000 67

1.0000 8.5000 1.7200 15.0000 64

1.0000 8.5000 1.7200 17.5000 62

1.0000 8.5000 1.7200 20.0000 63

1.0000 8.5000 2.1400 15.0000 68

1.0000 8.5000 2.1400 17.5000 67

1.0000 8.5000 2.1400 20.0000 65

The coefficients for the formation of hardness equation are,

107.2820

-4.5995

0.1873

-0.0889

Therefore, for AISI 10

Recommended

*View more*